EPS in CIVIL ENGINEERING APLLICATIONS: Product properties and performance requirements connected ABSTRACT Since decades expanded polystyrene (EPS) is successfully applied as light weight fill for roads railroads and other civil engineering applications. EPS is then often called “Geofoam”. Since 1st January 2009 a harmonised European product standard is in force, EN 14933, with the obligation of CE marking and labelling. Design in civil engineering was in most EU countries not subject to legal regulations but to guidelines, craftsmanship of engineers and common sense. From now on Eurocodes – especially EN 1997 EUROCODE 7 Geotechnical design - come into force which are equal for all EU countries (with some national application annexes). For simple constructions these two phenomena can easily connected via the stress – strain relationship.

MATERIAL PROPERTIES In this chapter the material properties of expanded polystyrene (EPS) are given for the calculation of EPS in geotechnical applications. The data correspond with the content of EN 14933 on compressive strength, modulus of elasticity and compressive creep. Compressive strength Short-term EPS product types are based on the declared value of the compressive strength at 10% deformation and has been an arbitrary choice. For the calculation of the design value of the short-term compressive strength σ10;d a material factor has to be taken into account (EN 1997 art 2.4.6.2 ); following EN 1990 and EN 14509 1 this factor (γm) is 1,25 (e.g. for EPS 100: σ10;d =100/1,25 = 80 kPa). This material factor is based on the steel sandwich panel standard supposing a variance of 8% in production of EPS, using a substantial amount of secondary materials. See: www.geoblock.nl Permanent strength As EPS is expected to have a compressive creep deformation of 2% or less after 50 years when subjected to a permanent compressive stress of less than 0,30 * σ10, the declared value of the permanent compressive strength σ10;perm = 0,30 * σ10. For the calculation of the design value σ10;perm;d the material factor (γm) has to be taken in to account (EN 1997 art 2.4.6.2); this factor (γm) is 1,25 (e.g. for EPS 100: σ10;perm;d = 0,3 * 100/1,25 = 24 kPa). Compressive strength under cyclic load On the basis of extensive studies it has been concluded that, with a relative light permanent loading at the top (15 kN/m2) and if the deformation under a cyclic load remains under 0,4% that deformation will be elastic and there will be no permanent 1

EN 14509, the European harmonized sandwich product standard

deformation. Translated into stresses the maximum safe value due to cyclic loading is 0,35 * σ10. This value has been recalculated from Duskov 2 thesis. Thus the declared compressive strength under cyclic load σ10;cycl;d = 0,35 * σ10 (e.g. for EPS 100: σ10;cycl;d =0,35 * 100 = 35 kPa). For the calculation of the design value σ10;cycl;d the material factor (γm) has to be taken in to account (EN 1997 art 2.4.6.2); this factor (γm) is 1,25 (e.g. for EPS 100: σ10;cycl;d = 35/ 1.25 = 28 kPa). Modulus of elasticity Declared values can be derived using test results from EN 826 and are valid for the elastic part of the stress/strain curve. The same value can be used for the calculation of the dynamic behaviour due to cyclic loading. Values in the next table are based on the formula developed by Horvath3: Et = (0,45 ρ -3) mPa (e.g. for EPS 100 (with a density ρ of 20 kg/m3) this gives Et = 0,45 * 20 -3 = 6 mPa = 6000 kPa). This is a “safe” approach. The relationship between density and compressive strength ( “old” versus “new” product types) is defined in “Eumeps Product Types” in 2003; see: www.eumeps.org

Compressive creep In 1989 dr. ing. Norbert Krollmann4 made a first proposal to determine and calculate the effect of compressive creep of thermal insulating materials, by suggesting to take the “Findley equation” to predict long term effects -“for the first decades”- based on testing during a period of 667 days, the result taken over in EN 1606. For civil engineering applications a prediction over a longer period is necessary. The Swedish testing institute SP proposed another extrapolation equation for long term creep based on the lin-log method (“Struik”). This was discussed in the CEN working groups and concluded that the “Findley” equation gives conservative results where “Struik” gives only good results for the longer period. This has to do also with two effects: tests are always carried out with small samples whilst in reality EPS light weight fill is using big blocks and secondly EPS shows stiffening of the product matrix at longer exposure to loadings. Taking into account that EN 1606 is the official harmonised European test method and with the knowledge that the creep behaviour of EPS corresponds with the “Struik”method for extrapolation a specific declaration is given in the EPS standards in an informative annex. This information is in addition to the conservative extrapolation method following “Findley”. The information in the annex is also conservative but saves a lot of extra testing and costs to manufacturers.

2

Duškov, Milan: EPS as alight weight sub-base material; 1997 Delft NL Horvath, J.S.: Geofoam Geosynthetic, Horvath Engineering, 1995 Scarsdale USA 4 Krollmann, Norbert: CEN TC 88 WG 4 N31-N111 dated 890425 3

Rheological model EPS

Creep data published by the SP in Goteborg in 2001 and published in EUMEPS’ WHITEBOOK 2003 prove the above given data in EN 13163 and EN 14933: at 0,3 (or 0,35 for EPS 150) times the compressive strength at 10% strain (σ10) the creep will be around 2% and the initial deformation around 0,5%, thus the total deflection (εt = ε0 + εct ) will be 2,5% over 50 years at a permanent load of 0,3 σ10. The data in this chapter are very useful for practical calculations. This was already presented at the Global Insulation Conference in Berlin 2007.

Tabulated properties The above obtained values are put in the next matrix: Table 1: Design properties of EPS Property

EPS product type

Description

Symbol

Unit

EPS60

EPS100

EPS150

EPS200

EPS250

Declared value short-term

σ10

kPa

60

100

150

200

250

σ10;d

kPa

48

80

120

160

200

Modulus of elasticity

Et; Edyn

kPa

4000

6000

8000

10000

12000

Declared value permanent

σ10;perm

kPa

18

30

45

60

75

σ10;perm;d

kPa

14,4

24

36

48

60

σ10;cycl

kPa

21

35

52,5

70

87,5

σ10;cycl;d

kPa

17

28

42

56

70

compressive strength Design value short-term compressive strength

compressive strength Design value permanent compressive strength Declared value compressive strength under cyclic load Design value compressive strength under cyclic load

PERFORMANCE REQUIREMENTS Geotechnical design

Only an integral approach of the design makes that design to a successful one – not only regarding its fitness for purpose or use but also in terms of sustainability and socioeconomic parameters. For this kind of road building anyhow the solution can be split up into three partial calculations. Most of the roads and railroads built on EPS use the equilibrium method: with bad subsoil and the possibility to avoid almost any settlements the concept with EPS is designed. For the subsoil the calculation method is than easy: as long as the permanent imposed load does not exceed the existing stresses zero settlements are to be expected. In case an load on the existing foundation is imposed well known calculations can follow to designate the settlements. For the load distributing top layer also tools are available to calculate the different layers in order to get a predicted equally distributed load on the EPS body. For difficult constructions software like PLAXIS can be used; for simple ones several Pavements Manuals exist. A lot of nonofficial, voluntary design rules in the EU are used (e.g. BAST, CROW and NRRL guidelines). Anyhow Eurocodes EN 1990 up until EN 1997 come into force and that means that the known calculation route via safety factors is left and the modern method with loading factors is more and more used. In this document general rules are described as a help to design simple civil engineering applications with EPS.

Loadings and combinations The given values are in conformity with EN 1990 and EN 1997 (Eurocode 7). Permanent loadings Permanent loadings of own weight and imposed dead loads can be derived from Eurocodes; for EPS a design value of 100 kg/m3 is taken into account “for possible water uptake” but the total load is small in comparison with sand, gravel and soil. For a light weight top layer 15 kPa can be taken. Traffic loads Traffic (cyclic) loads can be derived from Eurocodes. For the calculation of the EPS body in the Netherlands we often apply a uniform distributed load of 15 kPa thus already taken the load distribution by the gravel/ sand top layers and the bitumen reinforcement into account. Loading factors For permanent loads a loading factor of γF;G = 1,35 has to be applied; for traffic load a loading factor of γF;Q = 1,50 has to be applied (see EN 1997 Annex A3 Table A3 Collection A1); in case of the possibility of floating on ground water other factors have to be used.

Design criteria The following design criteria can be taken from EN 1990 to EN 1997: Ultimate Limit state short term criterion (“STR”) Loading combination: Multiply the dead and imposed load with their respective loading factors and combine both loads. Calculate the acting design compressive stress at the top of the EPS blocks and compare it with the short term design compressive strength σ10;d (e.g. 80 kPa for EPS 100). The short term acting stress should be less than or equal to the short term strength. Ultimate Limit state permanent criterion (“STR”) Loading combination: Multiply the dead load and the permanent part of the imposed load (mostly zero in civil applications) with their respective loading factors and combine both loads. Calculate the acting design compressive stress and compare it with the permanent design strength σ10;perm;d (e.g. 24 kPa for EPS100). The permanent acting stress should be less than or equal to the permanent strength. Ultimate Limit state for cyclic loads (“GEO”) Loading: Multiply the cyclic load with the factor γQ = 1,50. Calculate the acting design compressive stress and compare it with the design cyclic strength σ10;cycl;d (e.g. 24 kPa for EPS100). Note that a maximum dead load of 15 kPa is aalowed. Ultimate Limit state for floating (“UPL”) See for this Annex A4 of Eurocode 7; the load factor γG;stb = 0,9 in favourable situations and γG;dst = 1,0 in unfavourable situation for permanent actions. Load factor γQ;dst = 1,5 in unfavourable situation for variable actions. Limit state during the construction phase A worst case scenario has to be taken, no further defined criteria.

EXAMPLE OF APPLICATION As an example a typical road in the “Polders’ in the western part of the Netherlands is taken. The road is constructed by removing the peat soil to a depth of around 1,5 m; adding EPS blocks to a height of 2 m, putting a sand/gravel combination over it to distribute the point loads; it is finished with a double asphalt layer.

Permanent loads (γ=1,35) 0,15 m asphalt bitumen layers 0,15 * 2100 kg/m3 = 3,1 kN/m2 0,50 m gravel/sand 0,50 * 1800 kg/m3 = 9,0 kN/m2 2,0 m EPS 100 2,00 * 100 kg/m3 = 2,0 kN/m2 TOTAL = 14,1 kN/m2 Traffic load (γ =1,50) Cyclic and uniformly distributed on EPS = 15,0 kN/m2 STR- short: 1,35 * 14,1 + 1,50 * 15 = 41,35 < 80 ? O.K. STR-permanent 1,35 * 14,1 = 19,05 < 24 ? O.K. GEO-Cyclic 1,50 * 15 = 22,50 < 28? O.K. Conclusion: The product properties of EPS 100 fulfil the performance requirements 05-10-2009/tpr

http://www.stybenex.nl/files/STY090929ART-Tpr-EPS%20in%20CEA%20Mat%20prop%20and%20perf%20req%20conne

Published on May 10, 2010

http://www.stybenex.nl/files/STY090929ART-Tpr-EPS%20in%20CEA%20Mat%20prop%20and%20perf%20req%20connected.pdf

Advertisement